| ||Format||Pages||Price|| |
|PDF Version||9||$42.00||  ADD TO CART|
|Print Version||9||$42.00||  ADD TO CART|
|Standard + Redline PDF Bundle||18||$50.40||  ADD TO CART|
This practice covers the examination procedures for the contact, pulse-echo ultrasonic examination of heavy steel forgings by the straight and angle-beam techniques. An ultrasonic, pulsed, reflection type of instrument shall be used and shall provide linear presentation for at least 75% of the screen height. The 5% linearity referred to is descriptive of the screen presentation of amplitude. The electronic apparatus shall contain an attenuator, search units, transducers, couplants, reference blocks, and DGS scales. The forging shall be machined to provide cylindrical surfaces for radial examination in the case of round forgings. The ends of the forgings shall be machined perpendicular to the axis of the forging for the axial examination. Faces of disk and rectangular forgings shall be machined flat and parallel to one another. The procedures to be performed are as follows: ultrasonic examination of the forgings; straight-beam examination with establishment of the instrument sensitivity and calibration either by the reflection, reference-block technique, or DGS method; and angle-beam examination used for rings and hollow forgings.
This abstract is a brief summary of the referenced standard. It is informational only and not an official part of the standard; the full text of the standard itself must be referred to for its use and application. ASTM does not give any warranty express or implied or make any representation that the contents of this abstract are accurate, complete or up to date.
Significance and Use
This practice shall be used when ultrasonic inspection is required by the order or specification for inspection purposes where the acceptance of the forging is based on limitations of the number, amplitude, or location of discontinuities, or a combination thereof, which give rise to ultrasonic indications.
The ultrasonic quality level shall be clearly stated as order requirements.
1.1 This practice covers the examination procedures for the contact, pulse-echo ultrasonic examination of steel forgings by the straight and angle-beam techniques. The straight beam techniques include utilization of the DGS (Distance Gain-Size) method. See Appendix X3.
1.2 This practice is to be used whenever the inquiry, contract, order, or specification states that forgings are to be subject to ultrasonic examination in accordance with Practice A388/A388M.
1.3 Supplementary requirements of an optional nature are provided for use at the option of the purchaser. The supplementary requirements shall apply only when specified individually by the purchaser in the purchase order or contract.
1.4 The values stated in either SI units or inch-pound units are to be regarded separately as standard. The values stated in each system may not be exact equivalents; therefore, each system shall be used independently of the other. Combining values from the two systems may result in non-conformance with the standard.
1.5 This specification and the applicable material specifications are expressed in both inch-pound units and SI units. However, unless the order specifies the applicable “M” specification designation [SI units], the material shall be furnished to inch-pound units.
1.6 This standard does not purport to address all of the safety concerns, if any, associated with its use. It is the responsibility of the user of this standard to establish appropriate safety and health practices and determine the applicability of regulatory limitations prior to use.
2. Referenced Documents (purchase separately) The documents listed below are referenced within the subject standard but are not provided as part of the standard.
A469/A469M Specification for Vacuum-Treated Steel Forgings for Generator Rotors
A745/A745M Practice for Ultrasonic Examination of Austenitic Steel Forgings
E317 Practice for Evaluating Performance Characteristics of Ultrasonic Pulse-Echo Testing Instruments and Systems without the Use of Electronic Measurement Instruments
E428 Practice for Fabrication and Control of Metal, Other than Aluminum, Reference Blocks Used in Ultrasonic Testing
E1065 Guide for Evaluating Characteristics of Ultrasonic Search Units
Other DocumentRecommendedPracticef (1988 or later) Available from the American Society for Nondestructive Testing, 1711 Arlingate Ln., P.O. Box 28518, Columbus, OH 43228-0518.
ICS Number Code 77.040.20 (Non-destructive testing of metals); 77.140.85 (Iron and steel forgings)
UNSPSC Code 31132100(Steel forgings)